The Effects of Laser Forming on NiTi Superelastic yly1/PDFs/andrew 111.pdfThe Effects of Laser...
Embed Size (px)
Transcript of The Effects of Laser Forming on NiTi Superelastic yly1/PDFs/andrew 111.pdfThe Effects of Laser...
Andrew J. Birnbaum
Y. Lawrence Yao
Department of Mechanical Engineering,Columbia University,New York, NY 10027
The Effects of Laser Forming onNiTi Superelastic Shape MemoryAlloysThis work focuses on application of the laser forming process to NiTi shape memoryalloys. While all NiTi shape memory alloys exhibit both superelasticity and the shapememory effect, this study is restricted to a temperature range over which only the super-elastic effect will be active. Specifically, this work addresses laser forming induced mac-roscopic bending deformations, postprocess residual stress distributions, and changes inmicrostructure. Like traditional ferrous alloys, the laser forming process may be used asa means for imparting desired permanent deformations in superelastic NiTi alloys. How-ever, this process, when applied to a shape memory alloy also has great potential as ameans for shape setting memorized geometric configurations while preserving optimalshape memory behavior. Laser forming may be used as a monolithic process, whichimparts desired deformation while maintaining desired material behavior. Characteriza-tion of the residual stress field, plastic deformation, and phase transformation is carriedout numerically and is then subsequently validated via experimental results.DOI: 10.1115/1.4000309
Shape memory materials due to their highly specialized ther-omechanical behavior have received much attention in recent
ears. These behaviors include the traditional one way shapeemory effect SME, the superelastic effect, and the two-way
hape memory effect TWSME. The mechanism for all three be-aviors is rooted in the phase transformation properties of thelloy. The phase transformation may be induced via the applica-ion of an external load and/or a change in the alloy temperature.
Laser forming LF is a nontraditional manufacturing processhose effects have been extensively characterized at various size
cales for an array of materials and alloy systems. The mechanismor deformation is the generation of a transient nonuniform tem-erature distribution driving local thermal expansion and resultingn controllable permanent deformations. Although some workave been conducted on several classes of materials, the vast ma-ority of investigations are restricted to process application forerrous alloys 13.
NiTi shape memory alloys are typically produced by eitheracuum induction melting VIM or vacuum arc remelting VARn order to get a homogeneous nickel-titanium alloy constitution.he solidified ingots are then usually hot-worked when large ma-
erial reductions are required and then cold-worked and annealedn order to get the final product shape, surface finish, refined mi-rostructure, and mechanical properties 4,5. For most applica-ions, however, shape memory parameters, e.g., phase transforma-ion temperature, recoverable stress, and strain are not acceptablet this stage. An extra mechanical/heat treat step known as shapeetting are required to optimize these parameters with respect tohe desired memorized shape. Shape setting of shape memorylloys typically consists of constraining the cold-worked semifin-shed part in a desired configuration while subjecting it to anppropriate heat treatment in order to achieve the desired parteometry, superelastic, and/or shape memory behavior. Thisethod is limited in that the initial ingot geometry, as well as the
Contributed by the Manufacturing Engineering Division of ASME for publicationn the JOURNAL OF MANUFACTURING SCIENCE AND ENGINEERING. Manuscript receivedovember 10, 2006; final manuscript received December 15, 2008; published online
uly 21, 2010. Assoc. Editor: Kornel F. Ehmann.
ournal of Manufacturing Science and EngineeringCopyright 20
om: http://manufacturingscience.asmedigitalcollection.asme.org/ on 08/02
final desired geometry, must be fairly simple and requires thedesign and construction of part-specific fixturing.
The laser forming process avoids these limitations as it relies onthermal rather than direct mechanical means for deformation. Italso eliminates the need for hard tooling such as dies and fixtures.Furthermore, due to the inherent local and flexible nature of theprocess, it may be applied to simple as well as relatively complexinitial geometries, as outlined by Cheng and Yao 6.
Besides the ability to form parts with desired final geometries,the laser forming process has recently been shown to have poten-tial as a means for training the two-way shape memory effect 7.The two-way shape memory effect is characterized by a materialsability to remember two distinct configurations. Von Busse et al.showed that through multiple pulsed laser forming of NiTi thinfoils, one could train the formed part to have two distinct con-figurations that may be activated solely by thermal means. Laserprocessing of NiTi shape memory alloys SMAs have also re-cently received attention as a means for thin film deposition 8,laser induced actuation 9, laser annealing 10, and laser ma-chining of NiTi SMA components 11.
2 Process ConsiderationsWhile all NiTi shape memory alloys exhibit both superelastic
and shape memory effects, this study is restricted to a temperaturerange over which only the former will be active. Specifically, thiswork addresses laser induced macroscopic bending deformations,postprocess residual stress distributions, and microstructural andconsequences for the phase transformation.
The two prevalent phases exhibited in NiTi shape memory al-loys are the high temperature BCC Austenitic or parent phase,and the low temperature martensitic phase with lower symmetryB19 monoclinic crystal structure. The thermally induced phasetransformation is initiated by heating or cooling the material toabove or below the respective phase transformation temperatures.The temperatures at which the alloy will be fully austenitic ormartensitic are Af and Mf, respectively. The stress induced phasetransformation occurs over temperatures exceeding the austeniticfinish temperature accompanied by the application of a load suchthat the critical stress required for transformation is achieved re-sulting in the formation of a stress induced martensite SIM. This
is typically performed at temperatures greater than Af; therefore,
AUGUST 2010, Vol. 132 / 041002-110 by ASME
he initial composition of the alloy is completely austenite. Uponeleasing the load, the reverse transformation occurs resulting inomplete elastic recovery. Elastic strains of up to 89% have beeneported 12. The so-called R-phase characterized by a rhombo-edral microstructure also coexists as a transitional phase duringhe austenite to martensite transformation 13.
The stress/strain response of an austenitic superelastic NiTi al-oy is shown in Fig. 1 14. It is seen that upon loading there exists
linear elastic regime with an austenitic Youngs modulus fol-owed by a nonlinear portion whose start point at PT representshe onset of stress induced phase transformation. The range overhich this plateau spans is referred to as the transformation strain.ollowing this plateau, the sample is fully transformed into stress
nduced martensite. There then exists another linear elastic rangehat proceeds with the martensitic Youngs modulus followed bynother nonlinear portion representing the yield curve describingermanent slip and, finally, its ultimate tensile strength. PT cane determined via the ClausiusClapeyron relationship
nd is a positive function of temperature, where t, H, and Teq arehe transformation strain, enthalpy, and equilibrium phase trans-ormation temperature, respectively. The flow stress, y, of thelloy decreases with increases in temperature. These temperatureependencies become extremely relevant when describing aighly nonuniform thermomechanical process. In fact, at suffi-iently high temperatures, there is a temperature, Md, at which thetress to induce phase transformation is higher than that requiredor plastic deformation. At this point, the stress induced phaseransformation is no longer possible, and the constitutive responsef the alloy takes on the more traditional ferrous alloy appearanceith an elastic-plastic response. Figure 2 is a plot revealing the
rossover temperature for the alloy used in the presented experi-ents. The temperature dependence of the flow stress, as well as
he phase transformation stress, is obtained from literature 15.his crossover phenomenon adds a considerable amount of com-lexity to the process analysis, and the implications with respecto the laser forming process are discussed in the numerical ap-roach section.
Experimental Conditions and SetupExperiments were conducted with a CO2 laser with a maximum
500 W power output, with a Gaussian intensity distribution. Theaser system remained stationary while a precision XY stage trans-ated the specimens along the desired straight path and velocityFig. 3. The temperature gradient mechanism TGM, which is
ig. 1 Characteristic constitutive response of NiTi superelas-ic shape memory alloy in Af
ens were mechanically polished and then etched in a DIater:HNO3:HF, 5:2:1 solution. Figure 5 shows the as received
ntensity versus diffraction angle spectrum for the irradiated andntreated portion of the specimen provided by an Inel multipleetector X-ray diffractometer. These figures reveal that despite theeat treatment and annealing it has undergone, as well as its